- Research article
- Open Access
Development of a cartilage composite utilizing porous tantalum, fibrin, and rabbit chondrocytes for treatment of cartilage defect
© Jamil et al.; licensee BioMed Central. 2015
- Received: 11 September 2014
- Accepted: 14 January 2015
- Published: 7 February 2015
Functional tissue engineering has emerged as a potential means for treatment of cartilage defect. Development of a stable cartilage composite is considered to be a good option. The aim of the study was to observe whether the incorporation of cultured chondrocytes on porous tantalum utilizing fibrin as a cell carrier would promote cartilage tissue formation.
Rabbit articular chondrocytes were cultured and seeded onto tantalum with fibrin as temporary matrix in a composite, which was divided into three groups. The first group was kept in vitro while a total of 12 constructs were implanted into the dorsum of mice for the second and third groups. The implanted tissues were harvested after 4 weeks (second group) and after 8 weeks (third group). Specific characteristic of cartilage growth were studied by histological and biochemical assessment, immunohistochemistry, and quantitative PCR analysis.
Histological and biochemical evaluation of the formed cartilage using hematoxylin and eosin and Alcian blue staining showed lacunae chondrocytes embedded in the proteoglycan rich matrix. Dimethylmethylene blue assay demonstrated high glycosaminoglycans content in the removed tissue following 8 weeks of implantation. Immunohistochemistry results showed the composites after implantation expressed high collagen type II. Quantitative PCR results confirmed a significant increase in cartilage associated genes expression (collagen type II, AggC, Sox 9) after implantation.
Tantalum scaffold with fibrin as cell carrier promotes chondrocyte proliferation and cartilaginous tissue formation. Producing hyaline cartilage within a stable construct of tantalum and fibrin has a potential for treatment of cartilage defect.
- Cartilage composite
- Porous tantalum
- Chondrocyte proliferation
- Cartilage defect
Around two million individuals are affected worldwide with arthritis . These individuals require hospitalization, which is a matter of concern. Total joint replacement is the usual end-stage treatment, but implant longevity is an issue as more than half of the affected individuals is below 65 years old [2-7]. Damage to articular cartilage leads to premature arthritis. This chondral lesion was reported to be present in 60% of all patients aged between 40–50 years during arthroscopy [1,7,8]. Due to its avascular nature and ineffective response to injury, articular cartilage has limited potential to heal, even so in larger defects. Partial thickness injuries do not heal and merely stimulate minimal reaction to adjacent chondrocytes in the form of cell replication and matrix turnover, whereas full thickness injuries penetrating subchondral bone produce normal healing response but eventually fills the defect with fibrocartilage . Fibrocartilage resists to tension, in contrast to normal hyaline cartilage which resists compressive forces. Therefore, there is an urgent need for a method for effective biological healing and regeneration of cartilage to prevent premature arthritis.
There are various methods of operative treatment employed to treat osteochondral injury. Marrow stimulation and resurfacing techniques have been advocated but they have their limitations while dealing with large defects and producing hyaline cartilage [9-15]. Autologous chondrocyte implantation (ACI) which was brought into attention by Brittberg et al. in 1994 is quite promising but this technique is expensive and highly technically dependent . It requires two surgeries and needs laboratory support to grow the cells .
Functional tissue engineering is a novel approach to enhance tissue regeneration and provides the possibility of producing tissue that is biomechanically, biochemically, and histomorphologically similar to the native tissues . Scientists and engineers working in this promising field are taking steps to make those ideas a reality, working to supply biological substitutes or living tissue. A previous study by Munirah et al. for articular cartilage restoration focused on engineering autologous cartilage construct using human and ovine chondrocytes incorporated with the autologous fibrin as biomaterial . The pre-clinical study, conducted in sheep, was designed to evaluate the performance of the autologous ‘chondrocytes-fibrin’ construct implantation in a simulated clinical application prior to undertaking the definitive pre-clinical and clinical investigations. However, it has its own limitation. Resulted ‘chondrocytes-fibrin’ constructs were too soft to hold into the defect independently. Technically, periosteal patch were used to secure the implant into the defect.
There is continuous quest for the development of a new and more reliable technique to restore or reconstruct osteochondral defects. The development of a composite with the biochemical and mechanical properties of an osteochondral graft with better integration properties and without the need for autologous osteochondral graft harvesting or allogeneic tissue would be attractive. Tantalum, an elemental metal which is strong, biocompatible, and corrosive-resistant, has been widely used in the field of orthopedics due to its low modulus of elasticity and low frictional characteristics. It also has high, interconnected porosity with excellent bone in growth properties. In the present study, we incorporated cultured chondrocytes on porous tantalum utilizing fibrin as a cell carrier to support in vitro chondrogenesis. Following this, we compared it with constructs implanted for 4 and 8 weeks, which hypothetically has superior cartilaginous development.
The study was conducted after receiving the ethical approval from the animal and research ethics committee of our university. The project approval number from Universiti Kebangsaan Malaysia was FF-307-2009.
Chondrocyte cell preparation
Six New Zealand white rabbits age 2 months old and weighting 2.0–2.3 kilograms were used as experimental animals. Blood was taken to get autologous plasma and serum before the animal was sacrificed with overdosage of phenobarbital. Full-thickness cartilage was harvested from the knee, hip joints, and patella articular surface under aseptic technique. Each cartilage was separated from the perichondrium and subchondrium bone, minced into small pieces (1 mm3), washed with Dulbecco phosphate buffer saline (DPBS; pH 7.2; Gibco, Grand Island, NY, USA) containing 100 μ/ml penicillin and 100 μ/ml streptomycin (PBS, Gibco). Finally, the samples were washed with DPBS one more time. Cartilages were digested using 0.3% collagenase type II (Gibco) in a shaker incubator (Stuart Scientific, Redhill, UK) at 37°C for 90 min. Samples were centrifuged (500 × g) for 10 min to get the cell pellet. The supernatant was removed and the cell pellet was washed with 15 ml DPBS to remove the remaining enzyme. The sample was centrifuged for 10 min to get the final pellet cells. Isolated chondrocytes were seeded in six well plates containing the culture medium (Ham’s F12 and Dulbecco’s modified medium 1:1 + 1% ascorbic acid + 10% autologous serum + antibiotic/antimycotic + 1% glutamine). All cultures were maintained in 5% CO2 incubator (Jouan, Duguay, Trouin, SH) at 37°C with every 3 days medium change. Once confluence, the primary cultures were trypsinized using trypsin-EDTA 0.125% (Gibco). The cells pellet were then cultured in large-scale 175 cm2 culture flask (Falkon, Franklin Lake, NJ, USA) at a density of 5,000 cells/cm2. Chondrocyte morphologic features were examined every day using inverted light microscope (Olympus, Shinjukuku, Tokyo). Upon confluence, the cells were trypsinized and mix with plasma before put on to the tantalum. Fibrin polymerization took place after CaCl2 solution was added into the mixture. The cell-fibrin-tantalum constructs were maintained for 3 days in the culture before implantation. It was cultured in the same medium for cell expansion, in the six-well dishes and maintained in the CO2 incubator.
Harvest of composite
Three mice were sacrificed after 4 weeks and another three mice were sacrificed after 8 weeks to remove the constructs.
Histological and biochemical assessment
The obtained cartilage underwent histology and biochemical evaluation. Constructs were fixed in 10% formalin for 24 h at 4°C and processed using standard histological technique which finally embedded in paraffin. The tissues were cross sectioned (5 μm thick) and stained with hematoxylin and eosin, and Alcian blue according to standard procedures. For biochemical assessment, the amount of glucosaminoglycans (GAGs) was measured using the dimethylmethylene blue (DMMB) assay (12) and the total amount of GAGs per dry weight of formed cartilage (μg/ml/mg) was recorded.
For quantitative measuring of GAGs, the total GAGs content of cell/polymer constructs was determined using papain digestion and the dimethylmethylene blue dye method. Samples were lyophilized for 24 h and then digested under sterile conditions with papain type III (Sigma) at 125 mg/ml in a buffer of 0.1 M NaH2PO4, 5 mM methylenediaminetetraacetic acid, and 5 mM cysteine hydrochloride at pH 7.0 overnight at 60°C before the dye was added. Dimethylmethylene blue stock solution was made using dimethylmethylene blue, sodium chloride, glycine, sodium aziade in 1 N hydrochloride, and water. A spectrophotometer set at a wavelength of 520 nm was used to measure the optical density of the digested samples. Glycosaminoglycan was measured and reported in micrograms per milliliter per milligram of dry weight tissue.
Formalin-fixed tissues were sectioned and treated with proteinase K at 37°C for 60 min before washed three times with tris buffered saline (TBS, DAKO Cytomation). The sections were then treated with peroxidase block at 37°C for 10 min prior to incubation with antibody. Two antibodies were used, anti-type I and anti-type II collagen were diluted 1:150 with diluent (DAKO Cytomation) and applied to different sections for 40 min at 37°C. After washing with TBS, the sections were reacted with horseradish peroxidase (HRP) for 40 min at 37°C. After washing again with TBS, the signal was finally visualized as a brown reaction product from the peroxidase substrate 3,3′-diaminobenzidine (DAB).
Quantitative gene expression by real-time PCR
Total RNA was extracted from removed tissue engineered using TRI reagent (Molecular Research Center, Cincinnati) according to the manufacturer. Cartilage differentiation (type II collagen, SOX9 transcription factor, and aggrecan core protein), dedifferentiation (type I collagen), and hypertrophy (type X collagen) gene expression level was quantified by real-time PCR technique. Primer sequence used was designed with Primer 3 software based on the GeneBank database sequences corresponding to the specific gene Accession Number. The reaction kinetic and specificity of each primer set was verified with standard curve and melting profile. The quantitative RT-PCR protocol was performed in a Bio-Rad iCycler with profile of cDNA synthesis for 30 min at 50°C, pre-denaturation for 2 min at 94°C and PCR amplification for 38 cycles with 10 s at 94°C, 10 s at 60°C, and 30 s at 72°C. This series of cycles was followed by melt curve analysis to check the reaction specificity. The data was analyzed using Bio-Rad iCycler software. The expression level of each targeted gene was normalized to the house keeping gene - GAPDH.
Data for GAGs amount in each construct at all three environments (in vitro, in vivo, 4 and 8 weeks) were collected from 16 samples. Values were presented as mean ± standard error of mean (SEM). ANOVA and Student’s t test were used to compare data between groups. Differences were considered significant when p < 0.05. Data collected from quantitative parameter was analyzed using independent t test or Mann–Whitney test. Values were presented as mean ± SEM. Differences at 5% level were considered significant. All analyses were performed using SPSS 10.0 software.
Cellular morphology and construct gross appearance
GAG quantification of constructs
Quantitative comparison between in vitro and 4 weeks in vivo construct using Student t test demonstrated significant difference between the total amount of produced GAGs (p = 0.013). Comparison of total amount of GAGs per dry weight between 4 and 8 weeks in vivo demonstrated significant difference as well (p = 0.006). Samples at 8 weeks implantation formed more high-quality cartilage with higher amount of GAGs production.
Immunohistochemistry of constructs
Real-time PCR analysis on the constructs
Areas of research regarding cartilage repair have essentially focused on cultured cells supported in the engineered tissue. The delivery of this tissue is one of the challenges which include developing an appropriate scaffold and adhesive to provide matrix for the cells to grow. The term ‘chondroconductive’ was described by Gordon et al. and defined as providing a scaffold for the growth of cartilage and supporting structures . They found that porous tantalum is chondroconductive in vitro in dynamic environment. The potential of porous tantalum has been further evaluated by Mardones et al. in the development of cartilage-tantalum composite . In this study, periosteum from rabbits were placed on top of porous tantalum cylinders and cultured under chondrogenic conditions for 6 weeks. The findings show hyaline-like cartilage on the surface of the cylinders while the pores of the scaffold were filled with fibrous fixation. Mechanical testing was also performed which showed properties similar to normal rabbit cartilage. This cartilage from femoral condyles were made into osteochondral plugs and tested against the composite. It showed a stress–strain curve with characteristics typical of normal cartilage responding to a load. These findings have been the basis of further studies to consider cartilage-tantalum composite as an option for resurfacing and arthroplasty procedures. The abovementioned technique has limitation in term of making different thickness of cartilage from periosteum tissue. In the present study, we used fibrin to bind cultured chondrocytes and seeded onto tantalum in order to increase the feasibility of making various thickness of cartilage tissue.
The limitation of the study was the relatively short study period. An animal study by Shao et al. using allogeneic bone marrow mesenchymal stem cells (BMSC) seeded onto fibrin glue matrix and medical-grade polycaprolatone (mPCL) revealed deterioration of the transplant after 6 months, despite early good results . Admittedly, if the present study could have been conducted over the same time period with the previous reported study, we could have compared it better. Furthermore, the subcutaneous environment of our construct on the dorsum of nude mice might not be representative of a true clinical situation where intraarticular environment is involved. Mrosek et al. reported an in vivo study where cylindrical osteochondral defects were created on the medial and lateral condyles of ten rabbits and filled with tantalum/periosteum or poly-epsilon-caprolactone/periosteum biosynthetic composites . Even though subchondral bone regeneration was excellent, neo-cartilage formation from periosteum supported by a scaffold was inconsistent . However, Munirah et al. proved that autologous chondrocyte-fibrin construct (ACFC) promotes early chondrogenesis by inducing hyaline-like cartilage regeneration at 12 weeks post-surgery in a sheep model . Biomechanical testing is also appropriate as the next step for tantalum-chondrocyte-fibrin composite.
In the present study, the tissue-engineered cartilage showed morphological features of polygonal that became spindle-shaped and elongated during monolayer culture. These findings are similar to previous studies, which portrays the dedifferentiation in culture as the cultured chondrocytes lost their phenotype to adopt fibroblastic traits [15,21,22]. Our 2-month results also demonstrated that cultured chondrocytes within the fibrin and tantalum scaffold are able to differentiate and produce hyaline-like cartilage tissue. Histological evaluation of in vivo samples revealed chondroblast and chondrocytes surrounded by matrix containing hyaline. Seeded cell on tantalum in vitro was uniform and homogenous and contained immature chondrocytes with low concentration of GAGs in the hyalinized matrix, while in implanted constructs, the total amount of GAGs per dry weight of tissue significantly increased. This was further proven by strong immunopositivity by immunohistochemistry at 4 and 8 weeks, respectively. It also means that by 2 months, the cartilage has not featured any age-related changes yet. Studies with longer duration need to be done to evaluate the integrity of the cartilage. We also found that cartilage-associated genes (collagen type II, AggC, Sox 9) showed high gene expression after 8 weeks. This supports our hypothesis and suggested that the cartilage composite had produced a good matrix for the chondrocytes to differentiate. Similar findings were reported by previous studies of human articular chondrocytes [15,23]. Fibrocartilage and hypertrophic markers even though present showed much lower expression level. Sasano et al. also discovered that chondrocytes synthesize collagen type I and accumulate the protein in the matrix during his study of rat tibial articular cartilage [15,24].
These findings are in accordance with previous studies in proving that autologous chondrocyte and fibrin composite produced good-quality cartilage-like tissue [21,25-32]. In addition, we overcome the concern of fibrin glue detachment and degradation by providing a good scaffold with tantalum. Tantalum usage has been well established in clinical settings due to its biocompatibility and highly interconnected porosity which permits physiologic bone ingrowth and healing [17,33-41]. By 8 weeks, this tantalum-chondrocyte-fibrin composite show good promise in providing solution for cartilage defect. Clinically, this cartilage construct may be implanted arthroscopically and remain in situ with a stable scaffold. This advantage offers the option of a single surgery without the use of a periosteal patch which can be unstable.
We showed that tantalum scaffold with fibrin as cell carrier promotes cellular proliferation and cartilaginous tissue ormation of rabbit articular chondrocytes. Engineered cartilage resulted from in vivo-implanted construct demonstrated high-quality hyaline-like tissue by histological and biochemical assessment, GAG quantification, immunohistochemistry, and real-time PCR. This early results highlight the potential of tantalum-chondrocyte-fibrin composite in treatment of cartilage defect.
The source of funding for the study was from the Research Fund of Universiti Kebangsaan Malaysia. We would like to thank Professor Srijit Das for his help and contribution in completing the manuscript.
- Widuchowski W, Widuchowski J, Trzaska T. Articular cartilage defects: study of 25,124 knee arthroscopies. Knee. 2007;14:177–82.View ArticlePubMedGoogle Scholar
- Arden N, Nevitt MC. Osteoarthritis: epidemiology. Best Pract Res Clin Rheumatol. 2006;20:3–25.View ArticlePubMedGoogle Scholar
- Duffy GP, Trousdale RT, Stuart MJ. Total knee arthroplasty in patients 55 years old or younger. 10- to 17-year results. Clin Orthop Relat Res. 1998;356:22–7.View ArticlePubMedGoogle Scholar
- Duffy GP, Crowder AR, Trousdale RR, Berry DJ. Cemented total knee arthroplasty using a modern prosthesis in young patients with osteoarthritis. J Arthroplasty. 2007;22(6 Suppl 2):67–70.View ArticlePubMedGoogle Scholar
- Hofmann AA, Heithoff SM, Camargo M. Cementless total knee arthroplasty in patients 50 years or younger. Clin Orthop Relat Res. 2002;404:102–7.View ArticlePubMedGoogle Scholar
- Sheng PY, Konttinen L, Lehto M, Ogino D, J¨amsen E, Nevalainen J, et al. Revision total knee arthroplasty: 1990 through 2002. A review of the Finnish arthroplasty registry. J Bone Joint Surg Am. 2006;88:1425–30.View ArticlePubMedGoogle Scholar
- Wright TM, Maher SA. Current and novel approaches to treating chondral lesions. J Bone Joint Surg. 2009;91(1):120–5.View ArticlePubMedGoogle Scholar
- Shelbourne KD, Jari S, Gray T. Outcome of untreated traumatic articular cartilage defects of the knee: a natural history study. J Bone Joint Surg. 2003;85 suppl 2:8–16.PubMedGoogle Scholar
- Kakarlapudi TK, Bickerstaff DR. Articular cartilage lesions of the knee: putting the jigsaw puzzle together. Curr Orthop. 2002;16(2):139–50.View ArticleGoogle Scholar
- Brittberg M, Lindahl A, Nilsson A, Ohlsson C, Isaksson O, Peterson L. Treatment of deep cartilage defects in the knee with autologous chondrocyte transplantation. N Engl J Med. 1994;331(14):889–95.View ArticlePubMedGoogle Scholar
- Brittberg M, Tallheden T, Sjögren-Jansson B, Lindahl A, Peterson L. Autologous chondrocytes used for articular cartilage repair: an update. Clin Orthopaedics. 2001;391:337.View ArticleGoogle Scholar
- Gortz S, Bugbee WD. Allografts in articular cartilage repair. J Bone Joint Surg. 2006;88(6):1374.PubMedGoogle Scholar
- Knutsen G, Drogset JO, Engebretsen L, Grøntvedt T, Isaksen V, Ludvigsen TC. A randomized trial comparing autologous chondrocyte implantation with microfracture. Findings at five years. J Bone Joint Surg. 2007;89(10):2105.View ArticlePubMedGoogle Scholar
- O’Driscoll SW. Current concepts review: the healing and regeneration of articular cartilage. J Bone Joint Surg. 1998;80(12):1795–812.PubMedGoogle Scholar
- Sha’ban M, Soon HK, Ruszymah BH, Khang G. Fibrin and poly(lactic-co-glycolic acid) hybrid scaffold promotes early chondrogenesis of articular chondrocytes: an in vitro study. J Orthop Res. 2008;3:17.View ArticleGoogle Scholar
- Munirah S, Samsudin OC, Chen HC, Sharifah SH, Aminuddin BS, Ruszymah BH. Articular cartilage restoration in load-bearing osteochondral defects by implantation of autologous chondrocyte-fibrin constructs: an experimental study in sheep. J Bone Joint Surg Br. 2007;89(8):1099.View ArticlePubMedGoogle Scholar
- Gordon WJ, Conzemius MG, Birdsall E, Wannemuehler Y, Mallapragada S, Lewallen DG, et al. Chondroconductive potential of tantalum trabecular metal. J Biomed Mater Res. 2005;75(2):229–33.View ArticleGoogle Scholar
- Mardones RM, Reinholz GG, Fitzsimmons JS, Zobitz ME, An KN, Lewallen DG, et al. Development of a biologic prosthetic composite for cartilage repair. Tissue Eng. 2005;11(9–10):1368–78.View ArticlePubMedGoogle Scholar
- Shao XX, Hutmacher DW, Ho ST, Goh JC, Lee EH. Evaluation of a hybrid scaffold/cell construct in repair of high-load-bearing osteochondral defects in rabbits. Biomaterials. 2006;27(7):1071–80.View ArticlePubMedGoogle Scholar
- Mrosek EH, Schagemann JC, Chung HW, Fitzsimmons JS, Yaszemski MJ, Mardones RM, et al. Porous tantalum and poly-epsilon-caprolactone biocomposites for osteochondral defect repair: preliminary studies in rabbits. J Orthop Res. 2010;28(2):141–8.PubMedGoogle Scholar
- Idrus R, Chua KH, Munirah S, Noruddin N, Aminuddin BS. Tissue engineered cartilage with different human chondrocyte sources: articular, auricular and nasal septum. Med J Islamic World Acad Sci. 2005;15(1):5–12.Google Scholar
- Ishak MF, Chua KH, Asma A, Saim L, Aminuddin BS, Ruszymah BH, et al. Stem cell genes are poorly expressed in chondrocytes from microtic cartilage. Int J Pediatr Otorhinolaryngol. 2011;75:835–40.View ArticlePubMedGoogle Scholar
- Munirah S, Kim SH, Ruszymah BH, Khang G. The use of fibrin and poly (lactic-co-glycolic acid) hybrid scaffold for articular cartilage tissue engineering: an in vivo analysis. Eur Cell Mater. 2008;15:41–52.PubMedGoogle Scholar
- Sasano Y, Furusawa M, Ohtani H, Mizoguchi I, Takahashi I, Kagayama M. Chondrocytes synthesize type I collagen and accumulate the protein in the matrix during development of rat tibial articular cartilage. Anat Embryol. 1996;194(3):247–52.View ArticlePubMedGoogle Scholar
- Azmi B, Aminuddin BS, Sharaf I. The significance of using pooled human serum in human articular cartilage tissue engineering. Med J Malaysia. 2004;59:13.PubMedGoogle Scholar
- Chua KH, Aminuddin BS, Fuzina NH, Ruszymah BH. Interaction between insulin-like growth factor-1 with other growth factors in serum depleted culture medium for human cartilage engineering. Med J Malaysia. 2004;59:7.PubMedGoogle Scholar
- Chua KH, Aminuddin BS, Fuzina NH, Ruszymah BH. Human serum provided additional values in growth factors supplemented medium for human chondrocytes monolayer expansion and engineered cartilage construction. Med J Malaysia. 2004;59:194.PubMedGoogle Scholar
- Chua KH, Aminuddin BS, Fuzina NH, Ruszymah BH. Insulin-transferrin-selenium prevent human chondrocyte dedifferentiation and promote the formation of high quality tissue engineered human hyaline cartilage. Eur Cell Mater. 2005;9(9):58–67.PubMedGoogle Scholar
- Farah Wahida I, Aminuddin BS, Munirah S, Chua KH, Fuzina NH, Isa MR, et al. Gene expression characteristic in human auricular cartilage tissue engineering. Med J Malaysia. 2004;59:190.PubMedGoogle Scholar
- Munirah S, Aminuddin BS, Chua KH, Fuzina NH, Isa MR, Ruszymah BH. Tissue engineered human articular neocartilage using serial expanded chondrocytes. Med J Malaysia. 2004;59:9.PubMedGoogle Scholar
- Nur Adelina AN, Aminuddin BS, Munirah S, Chua KH, Fuzina NH, Saim L, et al. Phenotypic expression of collagen type II and collagen type I gene in monolayer culture of human auricular chondrocytes. Med J Malaysia. 2004;59:188.PubMedGoogle Scholar
- Saim L, Aminuddin BS, Munirah S, Chua KH, Izuddin Fahmy A, Fuzina NH, et al. Formation of tissue-engineered human auricular cartilage via tissue engineering technique for future use in ear surgery. Med J Malaysia. 2004;59:192.PubMedGoogle Scholar
- Bobyn JD, Stackpool GJ, Hacking SA, Tanzer M, Krygier JJ. Characteristics of bone ingrowth and interface mechanics of a new porous tantalum biomaterial. J Bone Joint Surg Br. 1999;81(5):907–14.View ArticlePubMedGoogle Scholar
- Cohen R. A porous tantalum trabecular metal: basic science. Am J Orthop. 2002;31(4):216–7.PubMedGoogle Scholar
- Garbuz DS, Hu Y, Kim WY, Duan K, Masri BA, Oxland TR, et al. Enhanced gap filling and osteoconduction associated with alendronate-calcium phosphate-coated porous tantalum. J Bone Joint Surg. 2008;90(5):1090.View ArticlePubMedGoogle Scholar
- Levine B, Sporer S, Della Valle CJ, Jacobs JJ, Paprosky W. Porous tantalum in reconstructive surgery of the knee: a review. J Knee Surg. 2007;20(3):185–94.PubMedGoogle Scholar
- Long WJ, Scuderi GR. Porous tantalum cones for large metaphyseal tibial defects in revision total knee arthroplasty: a minimum 2-year follow-up. J Arthroplasty. 2008;24(7):1086–92.View ArticlePubMedGoogle Scholar
- Macheras G, Kateros K, Kostakos A, Koutsostathis S, Danomaras D, Papagelopoulos PJ. Eight- to ten-year clinical and radiographic outcome of a porous tantalum monoblock acetabular component. J Arthroplasty. 2008;24(5):705–9.View ArticlePubMedGoogle Scholar
- Malkani AL, Price MR, Crawford 3rd CH, Baker DL. Acetabular component revision using a porous tantalum biomaterial: a case series. J Arthroplasty. 2008;24(7):1068–73.View ArticlePubMedGoogle Scholar
- Meneghini RM, Lewallen DG, Hanssen AD. Use of porous tantalum metaphyseal cones for severe tibial bone loss during revision total knee replacement. Surgical technique. J Bone Joint Surg Am. 2009;91(2):131–8.PubMedGoogle Scholar
- Patil N, Lee K, Goodman SB. Porous tantalum in hip and knee reconstructive surgery. J Biomed Mater Res B Appl Biomater. 2009;89(1):242–51.View ArticlePubMedGoogle Scholar
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.